Macromolecules 2005, 38, 3420-3425
Curvature Driven Flow of Thin Polymer Films and Diffusivity Measurements Ioannis Karapanagiotis*,† and William W. Gerberich‡ “Ormylia” Art Diagnosis Center, Ormylia, Chalkidiki 63071, Greece, and Department of Chemical Engineering and Materials Science, University of Minnesota, Minneapolis, Minnesota 55455 Received September 1, 2004; Revised Manuscript Received January 21, 2005
ABSTRACT: We study the leveling process of nanoindentation-induced defects on polystyrene (PS) films (h ) 100-150 nm) spin cast on silicon (Si) surfaces. Leveling occurs upon annealing above the glass transition temperature (Tg) of bulk PS, resulting in a flat polymer surface. The dynamics of the process is recorded with an AFM for PS molecular weights lower and comparable to the critical entanglement point. Diffusivity values measured from the recorded curvature driven flow are found to be in a very good agreement with corresponding self-diffusivity values of bulk PS.
Table 1. PS Properties: Radius of Gyration, Rg, and Surface Tension, γ, at 110 °C28
Wetting and dewetting of polymer coatings, thinner than a sessile drop flattened by gravity,1 have become major research topics,2-5 as polymer films find extensive applications in microelectronics, cultural heritage protection, and printing technology and are also used as membranes, adhesives, and paints. Within this framework, numerous investigations have been performed to study the stability of these films,6,7 whenever applied onto a hard nonwettable surface.8-12 For experimental studies, polystyrene (PS) film on silicon (Si) surface has been extensively utilized as a typical-model bilayer system for analogous investigations.10-18 It has been found that for films with film thickness (h) less than 100 nm dewetting occurs, upon heating above the glass transition temperature (Tg) of the polymer. In thicker films dewetting can be initiated only by, external, surface or interfacial defects.8,9,16,19 The (de)wetting dynamic evolution of thin films upon heating above Tg has been exploited to measure and investigate thin film properties such as density,20 viscosity,21,22 contact angle with the substrate,23,24 surface energy,25 and surface glass transition temperature.26 Following this spirit we have measured surface diffusivity values of low molecular weight (M ) 10 900 g/mol) PS by recording the leveling process of an indent induced by a probe on a PS film on Si as a function of temperature and found to be in relatively good agreement with the self-diffusivity of PS.27 In the present investigation, we examine this finding by keeping the annealing temperature constant (110 °C) and varying the molecular weight of the tested PS samples. Molar masses are shown in Table 1 along with the corresponding calculated radius of gyration (Rg) and surface tension (γ) of PS.28 A nanoindentation device, used typically to measure mechanical properties of films, was utilized to induce surface disturbances on PS films (h > 100 nm) on Si at room temperature. The residual depth of penetration (zD) was lower than the film thickness (zD < h). For thin †
“Ormylia” Art Diagnosis Center. University of Minnesota. * Corresponding author: e-mail [email protected]
; Tel 011 30 23710 98400; Fax 011 30 23710 98402. ‡
13 700 18 700 29 300 44 000
1.06 1.07 1.09 1.08
3.3 3.8 4.7 5.8
33.8 33.9 34.0 34.1
(h < 100 nm) films, these kind of defects can either grow toward the substrate and initiate dewetting or can heal level, resulting in a flat surface, upon heating above Tg.18 In the present study all indents healed. The leveling evolution was monitored using an atomic force microscope (AFM). In the following we first describe the materials and the experimental setup. We then provide a short description of the topographical changes that occur during an indent healing process. Considerations associated with the interactions that might contribute to this leveling process are then discussed. Curvature measurements in the thin regions (indents) are presented followed by diffusivity measurements. Finally, the effects (i) of the nanoindentation induced residual stresses and (ii) of the shear strain rate on the diffusivity measurements are evaluated. 2. Experimental Section Monodisperse PS with various molecular weights (Aldrich Chemical Co., Milwaukee, WI) shown in Table 1, was dissolved in spectroscopic grade toluene. Solutions of 5 wt % were applied onto 50 mm diameter silicon wafers (Virginia Semiconductor, Fredericksburg, VA) by spin-coating in a clean room of class 100. Samples were then dried in a vacuum chamber at 90 °C < Tg ()93 °C for Mw ) 13 700 g/mol) overnight. Ellipsometry was used to measure the thicknesses of the resulting films and found to be in the range 100-150 nm, depending on the molecular weight and spinning rate. The 〈100〉 oriented Si wafers were used as they were received by the supplier and contained a 1.7 nm thick native oxide layer. The resulting polymer films are expected to be unentangled (for PS Mc ) 38 000 g/mol), except for the samples produced by the 44 000 g/mol PS, which however does not differ substantially from the critical entanglement point.29 Nanoindents, with penetration depths lower than the film thicknesses, were imposed on the samples using a nanoindentation Hysitron Triboscope (Hysitron Inc., Minneapolis, MN) mounted with a standard three-sided pyramid (Berkovich)
10.1021/ma048216z CCC: $30.25 © 2005 American Chemical Society Published on Web 03/05/2005
Macromolecules, Vol. 38, No. 8, 2005
Curvature Driven Flow of Thin Polymer Films 3421
Figure 1. (a) Force-displacement curve of nanoindentation and (b) corresponding enlargement at point A showing the negative adhesive force developed between the indenter probe and a PS film. diamond tip of nominal radius of curvature 300 nm. The nanoindentation device adapts to an AFM which utilizes a Hysitron microsensor system instead of the standard AFM head component for applying loads electrostatically. The Hysitron Triboscope is a load controlled instrument. The loads required to induce shallow indents, with depths of penetration lower than the film thicknesses, were determined by preliminary experiments at which a series of nanoindentations were induced under different loads and imaged by AFM to measure the residual depths. The load range, finally used, was determined to be 230-270 µN. Deep indents, visible with an optical microscope, imposed under high forces (11 mN) served as markers to locate the indentation area and position the AFM tip at the vicinity of the shallow indents. Imaging was performed using a Nanoscope III SPM (Digital Instruments, Santa Barbara, CA) operated in the contact mode and mounted with a standard silicon nitride probe. Forces in the range of 1-10 nN were applied from the 200 µm cantilever to the polymer surface. Repeated scanning of the same surface area showed no alteration of the recorded topography due to the applied scanning force. The dynamics of the healing-leveling process of the imposed indents upon heating at 110 °C > Tg was recorded by AFM, following a cyclic procedure of heating at 110 °C and then quenching at room temperature and imaging. The evolution of each indent was monitored, for several anneal-quench cycles, before resulting in a flat surface identical to the rest of the free polymer surface. For all image acquisitions the same AFM probe was used.
3. Results and Discussion Leveling Process. Figure 1a shows a typical forcedisplacement (depth of penetration) curve obtained by
Figure 2. AFM images and corresponding cross sections showing the leveling process of a nanoindent, induced by a Berkovich tip, upon annealing for (a) 2.13, (b) 6.38, (c) 11.13, (d) 21, and (e) 33.25 min, at 110 °C. Point D corresponds to the maximum indent depth, defined as zD. The molecular weight of the PS film was Mw ) 18 700 g/mol.
a Hysitron triboscope, and Figure 1b is a magnification of the vicinity of point A at which the indenter tip withdraws from the sample. A negative force, shown in Figure 1b, corresponds to an adhesive, “pull-off” force between the diamond tip and the film. The presence of such force is indicative for soft, polymeric samples and suggests that the accurate measurement of the residual depth of penetration cannot be performed using loaddisplacement curves but requires imaging of the residual indent. Indentations, such as the one shown in Figure 1, resulted in indents with triangular top view shapes because of the three-sided pyramid (Berkovich) tip which was used for the nanoindentation tests.27 Upon heating above Tg, an indent evolves to circular. This (leveling) process is shown in Figure 2. The vertices and the sides of the initial triangle become round as the indent “expands” laterally, resulting gradually in a flat
Karapanagiotis and Gerberich
Macromolecules, Vol. 38, No. 8, 2005
Figure 3. Indent depth, zD, and maximum rim height, zR, normalized to their respective values at t ) 0 as a function of annealing time for PS with Mw ) 18 700 g/mol.
surface, similar to the rest of the free polymer surface.30 This evolution is accompanied by an increase of the surrounding rim width and indent diameter and an apparent decrease of the rim height and indent depth.27 Interactions Affecting the Leveling Process. From all the topographical changes occur during the healing-leveling process, described above, we focus in this study in the upward motion of the indent bottom, defined as point D in Figure 2. This motion is driven and can be affected by the following: (i) the mean curvature of the hole at the vicinity of point D, (ii) the relaxation of the surrounding rim, (iii) the van der Waals (VDW) interaction developed between the film and the substrate, (iv) the geometrical restrictions imposed by the small film thickness, and (v) the residual stress field induced by nanoindentation. Finally, one should evaluate also possible effects of shear rate on the leveling process, considering that the latter is recorded at a low temperature (110 °C) which is close to the Tg of bulk PS. The mean curvature effect is essentially the topic of this article and will be investigated in detail later. We will describe the dynamics of the hole healing process as a curvature driven flow. For a number of reasons that are provided below, the initial stages of the leveling process were not taken into account. In particular, diffusivity measurements were based on AFM images obtained after annealing the samples at 110 °C for more than ∼190 s. Images at the early annealing stages (annealing time